advertisement

EM388F Fracture Mechanics Term Paper Discussion of fracture criterions associated with the crack surface boundary conditions of piezoelectric materials By Rong Jiao Department of Aerospace Engineering and Engineering Mechanics 05/09/2008 1 Abstract: The fracture criterions of piezoelectric materials are different from those of common brittle and ductile materials due to their particular electrical-mechanical responses under the electrical-mechanical loading fields. There have five different fracture criterions for the crack in piezoelectric materials: (1) maximum loop stress; (2) total energy release rate (TERR); (3) mechanical strain energy release rate (MSERR); (4) local and global energy release rate only coming from the electrical yielding; (5) influence of mode-mixity on fracture. Using of these criterions is associated with the selections of the electrical boundary conditions including: (1) impermeable and mechanical traction free cracks surface; (2) permeable and mechanical traction free cracks surface; (3) exact electrical boundary and traction free cracks surface. In this term paper, two criterions (TERR and MSERR) under various mechanical and electrical loading fields for the impermeable crack surface and the permeable crack surface are discussed and for the impermeable crack, the mechanical strain energy release rate is reasonable while for the permeable crack, the total energy release rate is more reasonable. Introduction: In the last two or three decades, the piezoelectric materials have been used increasingly in the smart structures and adaptive technologies such as sensors, transducers and large displacement actuators. The most commonly used piezoelectric ceramics are PZT (PbZrO3-PbTiO3) and they are very brittle and very easy to induce fracture in its applications. So it’s important to study fracture behavior for the piezoelectric material and to discuss the reasonable fracture criteria for crack propagation. However, due to the particular electrical-mechanical responses under the electrical-mechanical loading, the fracture behavior of the piezoelectric ceramics is more complicated than those common materials which the Linear Elastic Fracture Mechanics can be used. In this term paper, two criterions (TERR and MSERR) under various mechanical and electrical loading fields for the impermeable crack surface and the permeable crack surface are discussed and for the impermeable crack, the mechanical strain energy release rate is a reasonable fracture criterion while for the permeable crack, the total energy release rate can be used as the fracture criterion. Fundamental fracture mechanics for piezoelectricity: Governing field equations: σ ij , j + f i = 0 (1) Di ,i = qb (2) There, σ ij is the stress tensor, f i is the body force and Di is the electric displacement, qb is the body charge. 2 Boundary conditions: σ ij n j = Ti (3) Di ni = − q s (4) There, Ti is the traction vector on the boundary, q s is the surface change and ni is the unit normal outward to the boundary surface. Constitutive equations, σ ij = Cijkl s kl − ekij E k (5) Di = eikl s kl + ε ik E k (6) There, C ijkl are the elastic modules, ε ij are the dielectric constants and ekij are the piezoelectric constants. For a generalized plane problem where all qualities in a 3D are not zero but they depends only on two Cartesian coordinates x1 and x 2 , Suo et al. (1992) developed Stroh’s complex potential theorem with four complex argument and gave a compact expressions form associated with the field equations (3) and the boundary conditions (4) as following: u = [u k , φ ] = af ( z ) , z = x1 + px 2 T (7) There, u k is the displacement and φ is the electric potential. f (z ) is an arbitrary function of the complex variable z and the complex constant p and the vector a are unknown currently and they can be solved out from the following eigen function: [Q + p(R + R T ] ) + p 2T a = 0 (8) The requirement of the non-trivial solution of equation (8) gives four pairs of complex conjugate eigen roots pα (α = 1,2,3,4) with the positive imaginary parts and the corresponding eigen vector a α (α = 1,2,3,4) . There, the matrix Q , R and T in equation (8) are related to the material mechanical, dielectric and piezoelectric constants in equation (5) and (6) by: ⎡C Q = ⎢ iT1k1 ⎣ e1k1 e1i1 ⎤ ⎡C , R = ⎢ iT1k 2 ⎥ − ε 11 ⎦ ⎣ e1k 2 e2i1 ⎤ ⎡C , T = ⎢ iT2 k 2 ⎥ − ε 12 ⎦ ⎣ e2 k 2 e2i 2 ⎤ − ε 22 ⎥⎦ (9) After given a particular expression of f (z ) , the stress and the electric displacement 3 can be gained: ⎧σ j 2 ⎫ ⎧σ j1 ⎫ T ' ' ⎨ ⎬ = (R + pR )af ( z ) ⎨ ⎬ = (Q + pR )af ( z ) D D ⎩ 2⎭ ⎩ 1⎭ (10) Or more compact forms from Suo et al. (1992): u = 2 Re[Af ( z )] (11) [σ i 2 ] = 2 Re[Bf ' ( z )] (12) [σ i1 ] = 2 Re[Lf ' ( z )] (13) With: u = [u1 , u 2 , u 3 , φ ] (14) [σ i1 ] = [σ 11 , σ 21 , σ 31 , D1 ]T , [σ i 2 ] = [σ 12 , σ 22 , σ 32 , D2 ]T (15) f ( z ) = [ f 1 ( z1 ), f 2 ( z 2 ), f 3 ( z 3 ), f 4 ( z 4 )] (16) T T A = [a1 , a 2 , a 3 , a 4 ] B = [b1 , b 2 , b 3 , b 4 ] , with b = (R T + pT)a (17) L = [− b1 μ1 ,−b 2 μ 2 ,−b 3 μ 3 ,−b 4 μ1 4 ] (18) Next, the solutions under the impermeable and permeable crack boundary conditions will be discussed. Impermeable crack surface: σ ∞ 22 x2 σ 12∞ D2∞ r θ 2a x1 Figure 1: The crack surface under the remote mechanical and electric loading Two surfaces of an impermeable crack are charge-free, or in the other words, the 4 normal components of dielectric displacement D2 along the crack surface are zero: + − D2 ( x ) = D2 ( x ) = 0 x ∈ ( − a, a ) (19) Just as we did in the Linear Elastic Fracture Mechanics, the mechanical quantities on the crack surfaces for the traction free conditions are: σ 12 + ( x) = σ 12 − ( x) = 0 , σ 22 + ( x) = σ 22 − ( x) = 0 x ∈ (−a, a) (20) By the same dimensional analysis used in LEFM, for the impermeable crack, the square root singularity still exists for both the stress and electric fields near the crack-tip. So, the crack-tip stress intensity factors (SIF) and the electric displacement intensity factor (EDIF) are associated with the remote mechanical and electric loading by: ∞ K I = σ 22 πa (21) K II = σ 12∞ πa (22) K e = D2∞ πa (23) From the expressions of equations (21-23), it’s evident that for an impermeable crack in an infinite plane piezoelectric material, the SIF’s do not depend on of remote electric loading D2∞ while EDIF does not depend on the remote mechanical loading σ 22∞ and σ 12∞ , neither. For the impermeable crack surface, the SIFs was suggested as a fracture criterion which is exactly we use in LEFM. But this is in contrary with the classical Vickers indentation experiments under an applied electric field, in which the fracture toughness dose depends on the electric field, may either decrease or increase, depending upon the direction of the applied electric field. So, SIFs is not a good fracture criterion for the impermeable crack since they do not consider the influence of the electric field on fracture. Park and Sun (1995) used the complex Fourier transformation to calculate the hoop stress near the crack-tip as function of angle θ for PZT-4 under the purely mechanical loading, pure electric loading and the combined mechanical-electric loading remote conditions, and the results are shown in Figure 2 and Figure 3. 5 Hoop Stress (Normalized) 30 20 10 0 -10 -20 -200 Only Stress33 Only D33 -100 0 100 200 Angle (Degree) Figure 2: Distribution of hoop stress at the tip of an impermeable crack under a purely mechanical or a pure loading (Park and Sun, 1995) Hoop Stress (Normalized) 6 4 2 D33(C/m2) 0 -2 -200 0 0.01 0.02 -100 0 100 200 Angle (Degree) Figure 3: Distribution of hoop stress at the tip of an impermeable crack surface under a combined mechanical and electric loading (Park and Sun, 1995) These two figures show that the angle θ for the maximum hoop stress is greatly influenced by the remote electric loading and we know that in the case of pure mechanical loading in LEFM, the maximum hoop stress is at θ = 0 . But here, this position is affected by the applied electric loading and maybe it’s not at θ = 0 . In LEFM, the J-integral is equivalent to the crack-tip energy release rate (ERR) per unit crack extension (also known as the total potential energy release rate, shortly by 6 TPERR) that includes both mechanical and electric energy. So, consequently, TPERR has been suggested to be used as the fracture criterion for piezoelectric material. J-integral can be calculated as follows; ⎡⎛ ∂u p ⎞ ⎛ ∂φ ⎞⎤ J = ∫ ⎢⎜⎜ σ ij sij dx 2 − niσ ip ds ⎟⎟ − ⎜⎜ Di Ei dx 2 + ni Di ds ⎟⎥ ∂x1 ⎟⎠⎥⎦ ∂x1 ⎠ ⎝ ⎢⎝ C⎣ i, j, p = 1,2 (24) There, C denotes the closed contour surrounding the crack tip and in the paper Suo et al (1992), the J-integral was associated with the SIFs by: ⎛ K II ⎞ ⎜ ⎟ 1 * J = ( K II , K I , K e )H ⎜ K I ⎟ 4 ⎜K ⎟ ⎝ e⎠ (25) There H * is a 3× 3 matrix and is related to the piezoelectric material constants as: −1 H * = 2 Re(iA * B * ) (26) ⎡ p1 A = ⎢⎢ q1 ⎢⎣ r1 (27) * ⎡ − μ1 B = ⎢⎢ 1 ⎢⎣ − λ1 * p3 ⎤ q1 ⎥⎥ r1 ⎥⎦ p2 q1 r1 − μ2 − μ3 ⎤ 1 ⎥⎥ − λ1 ⎥⎦ 1 − λ1 (28) In the paper of Park and Sun (1995), for the model-I crack normal to the poling direction and the applied electric field in PZT-4, the expression of TPERR was: πa ∞ 2 ∞ ∞ ∞ 2 (29) GI = 1.48 × 10 −11 (σ 22 ) + 5.34 × 10 − 2 σ 22 D22 − 8.56 × 10 7 ( D22 ) 2 In this expression, besides the mechanical part, the TPERR also includes the electric part and the coupling term of mechanical and electric loading. But the problem is the [ ] ∞ ∞ ∞ is negative, and consequently, for different σ 22 and D22 , the last term square D22 value of TPERR may be zero or even negative. So, for a fixed mechanical loading, use of the TPERR as the fracture criterion will always block crack propagation under an applied electric loading, whatever the direction of the applied electric loading is. Moreover, if there has no mechanical loading, a purely eclectic loading never drives the crack since the last term in equation (29) is always negative. These deductions obviously do not coincide with all available experimental observations and common sense. So, for the impermeable crack, the total energy release rate TPERR can not be used as the fracture criterion. So, Park and Sun (1995) used a new fracture criterion based on mechanical strain energy release rate (MSERR) since they believed that the fracture is a mechanical process and it’s more reasonable to only use the mechanical strain energy released during crack propagation. The MSERR is the crack closure integral for the mechanical 7 part, which can be defined as follows: δ G IM = lim 1 2δ ∫ G IIM = lim 1 2δ δ δ →0 δ →0 0 ∫ 0 σ 22 ( x)Δu 2 (δ − x)dx (Mode I) (29) σ 12 ( x)Δu1 (δ − x)dx (Mode II) (30) Also, Park and Sun (1995) proposed the expression of MSERR for an impermeable crack normal to the poling direction of PZT-4: πa ∞ 2 ∞ ∞ (31) G IM = 1.48 × 10 −11 (σ 22 ) + 2.67 × 10 − 2 σ 22 D22 2 Now from this expression, we found that the negative term disappears and the MSERR has the linear relationship to the remote eclectic loading under non-zero mechanical loading. Park and Sun found that a positive electric field decreases the critical stress at which the fracture occurs and hence accelerate crack growth while a negative electric field increases the fracture stress hence blocks crack growth. This conclusion matches the experiments they did very well, which is shown in the figure 4 and figure 5. 160 [ ] Center Crack Test GM Prediction Fracture Load (N) 140 120 100 80 60 -8 -4 0 4 8 12 Electric Field (kV/cm) Figure 4: Fracture load as a function of electric filed for a center crack in PZT-4 (Park and Sun, 1995) 8 180 2mm Off-Center Crack Test GM Prediction Fracture Load (N) 160 140 120 100 80 -8 -4 0 4 8 12 Electric Field (kV/cm) Figure 5: Fracture load as a function of electric filed for a 2mm off-center crack in PZT-4 (Park and Sun, 1995) By the comparison of the experiments and the prediction of G M , it is concluded that the MSERR is a better fracture criterion than the TPERR when the crack surface are charge-free. Park and Sun (1995) suggested that the charge-free crack surface can be obtained by putting a crack specimen in the silicone oil. Permeable crack model: In the impermeable crack model, the normal electric displacement and the corresponding electric potential are assumed zero. But actually, the magnitude of the normal electric displacement on crack surfaces does not vanish and they should be continuous through the two surfaces of the crack: + − D2 ( x1 ) = D2 ( x1 ) (32) φ 2 + ( x1 ) = φ 2 − ( x1 ) (33) For the permeable crack model, it’s significant to find the distributed normal eclectic 0 displacement D2 ( x1 ) which is the difference between the two surfaces of the crack. 0 It is found that under the uniform far-field loading, D2 ( x1 ) is constant. So, equation (33) is reduced to: + − E 2 ( x1 ) = E 2 ( x1 ) (34) Xu and Rajapakse (2001) found that the normal electric displacement on crack surfaces is related to the uniform far-field loadings by: 9 3 D2 = 0 ∞ Im ∑ κ k (− Ak1σ 22 + Ak 2σ 12∞ ) k =1 3 Im ∑ κ k Ak 3 + D2 ∞ (35) k =1 There, the constants κ k and Aki are related to equation (27). From equation (35), we found that as the complex coefficient in the complex potentials are not dependent ∞ ∞ to the remote electric displacement D2 itself, but the electric quantity D2 − D2 . 0 Also, Xu and Rajapakse (2001) proposed the following expression for the field intensity factors: ∞ K I = σ 22 πa (36) K II = σ 12∞ πa (37) K e = ( D2∞ − D20 ) πa (38) Here, for a conducting crack, the remote electric loading D2 ∞ has no influence on the complex potential solutions and this implies that for a conducting crack, the remote mechanical loading plays a much more significant role than the remote electric loading and consequently, the traditional mechanical SIFs may be used as a fracture criterion for conduction cracks. Xu and Rajapakse (2001) proposed the formula for the total potential energy release rate (TPERR) for a conducting crack including its mechanical and electric parts as following: G = G M + G E = lim δa →0 G M 1 δa {σ i 2 ( x,0)u i (δa − x,±π ) + D2 9 x,0)φ (δa − x,±π )}dx (39) 2δa ∫0 ∞ 2 ∞ ⎧⎪− q k Ak 1 (σ 22 ) + p k Ak 2 (σ 12∞ ) 2 + (q k Ak 2 − p k Ak 1 )σ 12∞ σ 22 Im ∑ ⎨ = 0 ∞ ∞ ∞ ∞ 2 k =1 ⎪ ⎩( p k Ak 3σ 12σ 22 + q k Ak 3σ 22 )( D2 − D2 ) GE = πa πa 2 3 3 { ∞ Im ∑ (− s k Ak1σ 22 + s k Ak 2σ 12∞ )( D2∞ − D20 ) + s k Ak 3 ( D2∞ − D20 ) 2 } + ⎫⎪ ⎬ ⎪⎭ (40) (41) k =1 Using this formulas, Liu and Chen (2002) analyzed the energy for both permeable and impermeable cracks in the piezoelectric materials and the numerical results of G M , G E and G are plotted in figure 6~8, respectively. 10 14 Red~Impermeable Blue~Permeable 12 E2=2.0e-3V/m E2=0 E2=-2.0e-3V/m 10 8 Stress22=0.6Mpa GM 6 4 2 0 -2 -4 -6 0 20 40 60 80 100 120 140 160 180 a(degree) Figure 6: Mechanical part of TPERR against the crack oriented angle (Liu and Chen, 2002) 0 -1 -2 -3 GE -4 -5 Red~Impermeable Blue~Permeable -6 E2=2.0e-3V/m -7 E2=0 -8 E2=-2.0e-3V/m Stress22=0.6Mpa -9 -10 0 20 40 60 80 100 120 140 160 180 a(degree) Figure 7: Electric part of TPERR against the crack oriented angle (Liu and Chen, 2002) 11 14 Red~Impermeable Blue~Permeable 12 E2=2.0e-3V/m E2=0 E2=-2.0e-3V/m 10 8 Stress22=0.6Mpa G 6 4 2 0 -2 -4 -6 0 20 40 60 80 100 120 140 160 180 a(degree) Figure 8: TPERR against the crack oriented angle (Liu and Chen, 2002) The mechanical part G M in the TPERR against the crack orientation angle α is always positive for the permeable crack. It’s interesting that under the pure mechanical loading ( E 2∞ = 0 ), the values G M of for the permeable crack are always bigger than those for the impermeable crack, which means that the permeable crack surface condition enhances the crack propagation compared with the impermeable characteristic. Under the mechanical-electrical loading, the values of G M is almost constant for the permeable crack irrespective of the applied electric loading and this implies that G M is independent of the electric loading under the situation of permeable crack boundary conditions. While for the impermeable crack, the mechanical strain release rate G M is influenced by the applied electric loading: compared with the value of G M under the pure mechanical loading, the positive electric loading increase G M while the negative decreases G M . In the figure 7, the value of G E is always zero for the permeable crack, which implies that is no electric energy release rate for the permeable crack boundary condition. This can explain that why TPERR criterion could be used as a fracture criterion for the permeable crack, since the electric part G E vanishes and mechanical part G M is overwhelming irrespective of the positive or negative electric loading. However, for 12 the impermeable crack, the applied electric loading influences on G E and due to the effect of the electric part of G E in TPERR, TPERR criterion can not be used for the impermeable crack. In this situation, by Park and Sun (1995), the mechanical strain energy release rate (MSERR) is a good choice. Conclusion: Several fracture criterions for the piezoelectric materials under impermeable and permeable boundary conditions are discussed here. For the impermeable crack, Park and Sun (1995) concluded that rather than the total energy release rate (TPERR), the mechanical strain energy release rate (MSERR) can be used as the fracture criterion; while for the permeable crack, TPERR is useful since the electric part G E is negligible. Reference: Chen YH and Lu TJ, 2003. Cracks and fracture in piezoelectrics. Advance in Applied Mechanics, 39:121–213 Liu Q. and Chen YH, 2002. Energy analysis for permeable and impermeable cracks in piezoelectric materials. International Journal of Fracture, 116: 15-20. Xu XL and Rajapakse R.K.N.D, 2001. on a plane crack in piezoelectric solids. International Journal of Solids and Structures, 38: 7643-7658. Suo, Z., Kuo, C. M., Branett, D. M., and Willis, J. R., 1992. Fracture mechanics for piezoelectric ceramics. Journal of the mechanics and physics of solids, 40, 739-765. Park, S. B., and Sun, C. T., 1995. Effect of electric fields on fracture of piezoelectric ceramics. International Journal of Fracture, 70, 203-216. 13